Continuous, monodisperse silver nanoparticles synthesis using microdroplets as a reactor
- 203 Downloads
In this paper precisely controlled silver nanoparticles synthesis method using microdroplets as a reactor was shown. It was confirmed that the application of microdroplets effects in a decrease in particles size and size distribution in comparison with a typical batch reactor from 4.8 ± 1.3 nm to 2.5 ± 0.5 nm. This decrease of particles size distribution is directly related to the fact, that thanks to the application of microdroplets as reactors the mass transfer limits were eliminated.
KeywordsDroplets Microreactor Silver nanoparticles DMAB
In the last decade, the synthesis of nanomaterials has made a large step forward, due to their potential application in many areas such as catalysis [1, 2], medicine [3, 4], optics , tissue , etc. Nanomaterials have due to their high surface to volume ratio  unique properties different from bulk materials such as optical [8, 9] and electronically  properties. Two methods are at hand for the synthesis of nanomaterials, i.e. physically  or chemical  based. Efficient nanomaterial syntheses provide particles of defined size, morphology, composition, performance property, etc. However, the choice of synthesis route depends on a few more factors: equipment cost, production intensity, type of reagents, and complexity of synthesis [13, 14]. Taking into account these factors, a commonly used protocol is the chemical reduction of metal precursor with reductant in an aqueous media. This chemical reduction can be conducted in batch reactor or in microreactor.
Microfluidic systems allow a particularly good process control. This is most evident from their ability to tune nanoparticle size, and narrow the nanoparticles size distribution [9, 10, 15, 16, 17, 18, 19, 20, 21, 22]. The high volume-specific ratio of channel surface area to volume enables ultrafast mixing and fast heat exchange which are of utmost relevance to the seed formation and particle growth. Essentially the same feature, however, also promotes adsorption of the formed nanostructures and such fouling can finally lead to system blocking.
In this paper we like to show the application of sequential flow for silver nanoparticles synthesis. Sequential flow comprises a chain of aqueous droplets in a moving continuous organic medium. Different from segmented flow, the droplets are smaller than the channel diameter and thus do not attach to the channel surface through a very thin liquid capping layer. Brutchey et al.  were investigating microfluidic droplet flows of ionic liquids for silver and gold nanoparticles synthesis. They have shown that the AuNPs synthesized in batch were 29% larger than those produced in the microfluidic device. Also Yang et al.  were investigating continuous flow process for silver nanoparticles synthesis. In both mentioned above papers, experiments were performed in non-aqua media. What probably makes these technologies more expensive in compere with water base systems.
In our previse paper , optimal conditions for droplet formation were investigated. From this study, essential process conditions for the droplet formation were determined like the phase composition and the flow rate.
In this paper, we proposed the application of a chain of droplets as a set of little reactors, which flows within a continuous phase, i.e. the sequential flow. We would like to check if it is possible to decrease the nanoparticles size distribution formed as compared to a typical batch reactor. We hope that the sequential flow might give similar advantages for nanoparticle synthesis as known for the segmented flow. For this a fast reaction reduction of silver(I) ions and a homogeneous process of nucleation and growth in all reaction volume will be needed.
Silver nanoparticle synthesis was performed using silver(I) nitrate(V) (AgNO3, Avantor Materials) as metal precursor. A stock solution containing Ag+ ions was prepared as follows: 16.987 g of AgNO3 was dissolved in 0.1 M of HClO4 (Avantor Performance Materials, P.A) to finally obtain 0.1 mol/dm3 solution. This solution was stored in brown glass bottle. Borane dimethylamine complex 97% (DMAB, Fluka) was used as the reducing agent. Heptane (Avantor Materials, P.A), was used as oil phase. Span 80 (delivered by Sigma Aldrich), polyvinyl alcohol (PVA, Sigma Aldrich, MW = 67,000) and Tween 80 (Avantor Performance Materials, P.A) were used as surface active agents to obtain stable and homogeneous droplets. The last two polymers (PVA and Tween 80) may also act as silver nanoparticle stabilizing agents.
In all experiments concerning the application of the two phase system (in this paper termed as heterogeneous system), the water phase consists of 1% PVA(m/v ratio) and 1% of Tween80 (v/v ratio). The concentration of Ag+ ions was equal to 2 × 10−4 mol/dm3, and the oil phase consists of heptane and 1% of Span80 (v/v).
In case of the homogenous system, all reagents were dissolved in water. Since Span 80 is insoluble in water, this polymer was not applied. For this purpose two solutions were prepared. The first one, contains the reductant (20 mmol/dm3 of DMAB), and 1%PVA (m/v) and 1% of Tween80 (v/v). The second one, comprising the precursor was prepared by dilution of stock solution of Ag+ in water to finally obtain concentration of Ag+ equal to 2 × 10−4 mol/dm3 and 1%PVA(m/v) and 1% of Tween80(v/v). Next, those two solutions were mixed in a volume ratio 1:1 to obtain AgNPs. This set of experiments is termed as homogeneous system.
To obtain low flow pulsation during the silver nanoparticles synthesis, syringe pumps (Injectomat Agilla, Fresenius Kabi) were used.
HR-TEM analysis was performed using the instrument (HR – TEM) – FEI TECNAI TF 20 X-TWIN. For this purpose, one drop of freshly prepared colloidal suspensions was placed on a copper grid covered by a 20–30 nm amorphous carbon film. Then, the samples were left to dry at room temperature (c.a. 20 °C).
The zeta potential of the obtained material as well as the size and size distribution were determined using the Zetasizer Nano ZS (Malvern Instrument). For this purpose, a standard clear polycarbonate cell with gold electrodes was used.
UV-Vis spectra were registered using the Shimadzu model U-2501 PC. 10 mm and 2 mm path length quartz cuvettes were used for the analysis, and base-line corrected against the reference water filled quartz cuvette.
XRD analysis was performed using an X − ray diffractometer (Rigaku MiniFlexII). For this purpose, ca. 5 mL of the obtained colloidal sample was slowly evaporated on the holder surface. Next, the analysis was performed.
Experimental conditions of the silver nanoparticle synthesis and microchannel flow configuration
The silver nanoparticle synthesis was performed in two different reactor systems which are homogeneous (water) phase in a batch reactor and the microdroplets reactor. The synthesis conditions have been kept identical in all cases, concerning the reductant and precursor concentration, temperature, and the stabilizing agents addition. In that way, it is ensured that all kinetically relevant parameters have been set the same, and thus reaction kinetics are the same. As there is then also no heat transport issue, only mass transport through diffusion can have impact on the particles size and size distribution. The process of silver nanoparticle formation in microdroplets was conducted in a microreactor, taking into account the results (flow rate conditions) obtained in our previous study , in which it the common sense was followed that increasing mixing rate (up to elimination of diffusion) can lead to the formation of monodisperse particles.
The flow rate of the oil phase was equal to 5 mL/h, and the flow rate of the water phase was equal to 1 mL/h .
It can be seen (Fig. 1), that for the selected flow condition, the formed droplets (water phase) are uniform in size and shape.
It should be underlined that the water droplets das not have a contact with the reactor walls during silver nanoparticles synthesis reaction. This effective avoid the system blocking.
Results and discussion
Figure 2b shows the colloidal silver obtained in the two phase system (microdroplets) with the reductant and precursor in the water phase. The color of the sample is much lighter compared to those shown in Fig. 2a.
Particle size and size distribution obtained in batch and microdroplets reactor
Average particles diameter *, nm
Size deviation, nm
Zeta potential, mV
−5.1 ± 6.8
Homogenous system in micro droplets
−14.7 ± 5.8
For all colloids, the values of the zeta potential were registered and are also depicted in Table 1. It was observed, that the zeta potential changes from -5 mV for the reaction reduction of Ag(I) ions with DMAB when being conducted in the homogeneous system in the batch reactor up to −14.7 mV for reaction when being conducted in microdroplets.
HR-TEM image of the sample obtained in the batch reactor is shown in Fig. 4a. In part B of this figure particle size histogram is shown. As it can be seen, there is an excellent agreement between results obtained using DLS and TEM method.
In the case of the AgNPs synthesized in microdroplets, a significant decrease of particle size and size distribution was observed. The crystallography analysis showed only FCC structures (see fig Fig. 5a and b). In part C of this figure particle size histogram is also shown.
Two broad peaks can be observed which are actually composed of two elemental peaks. The significant broadening of those peaks relates to the nanocrystalline structure.
is the mean size of the crystalline, nm
is the shape factor, in this case assumed as 0.94, A.U.
is the X-ray wavelength, in this case equal to 0.15418, nm
is the fitted peak broadening at half the maximum (FWHM), rad
is the Bragg angle, rad
In Fig. 6 B the deconvolution of the selected peak with the highest intensity is shown. It is known that this peak should consist of two elemental subpeaks with maximum at 38.1 for the crystallographic plane (1,1,1) and 44.37 for the crystallographic plane (2,0,0). The numeric analysis reveals that the FWHM equals to 8.6 o and 9.3o respectively. Taking above into account the crystalline mean size was calculated to equal 1.02 and 0.96 nm respectively. This in turn suggests that there is no shape anisotropy, what is in good agreement with the HR-TEM analysis. Moreover, it confirms the observation of a polycrystalline structure for the obtained nanoparticles.
Summary and conclusion
In this paper, we have shown, that the polydispersion of nanoparticles is associated with diffusion limit during synthesis. Improvement of mixing during the reaction leads to a decrease of particles size and size distribution. In microdroplets, the gradient of concentration of reagents is eliminated much faster than in a typical batch reactor. Even, microflow reactors are limited since mixing is mainly controlled by diffusion. In the case of microdroplets, interphase friction is a driving force for mixing. It was observed that thanks to the application of microdroplets effective size of nanoparticles were decreased from 4.8 ± 1.3 nm to 2.5 ± 0.5 nm.
It should be noted, that the application of two-phase flow, allowed to not only control the particles size distribution but also, prevent from nanoparticles deposition at the walls of the microreactor. During our experiments, the whole setups were working continuously 12 h without visible effects of nanoparticles deposition on the walls of the microreactor.
It is expected that the observed effect can be reproducible regarding the size and uniformity of other metallic nanoparticles such as gold, platinum, palladium or even semiconductors such as TiO2 or ZnO.
This study was funded by the Polish Ministry of Science and Education (grants no IP2014051773 Iuventus Plus).
Compliance with ethical standards
Conflict of interest
The authors declare that they have no conflict of interest.
- 1.Wojnicki M, Luty-Błocho M, Dobosz I, Grzonka J, Pacławski K, Kurzydłowski K, Fitzner K (2013) Electro-oxidation of glucose in alkaline media on graphene sheets decorated with gold nanoparticles. Mater Sci Appl 4(2):162–169Google Scholar
- 4.Bednarski M, Dudek M, Knutelska J, Nowiński L, Sapa J, Zygmunt M, Nowak G, Luty-Błocho M, Wojnicki M, Fitzner K, Tęsiorowski M (2015) The influence of the route of administration of gold nanoparticles on their tissue distribution and basic biochemical parameters: in vivo studies. Pharmacol Rep 67(3):405–409CrossRefGoogle Scholar
- 6.Terentyuk GS, Maslyakova GN, Suleymanova LV, Khlebtsov BN, Kogan BY, Akchurin GG, Shantrocha AV, Maksimova IL, Khlebtsov NG, Tuchin VV (2009) Circulation and distribution of gold nanoparticles and induced alterations of tissue morphology at intravenous particle delivery. J Biophotonics 2(5):292–302CrossRefGoogle Scholar
- 11.Iravani S, Korbekandi H, Mirmohammadi SV, Zolfaghari B (2014) Synthesis of silver nanoparticles: chemical, physical and biological methods. Res Pharm Sci 9(6):385–406Google Scholar
- 14.Makgwane P, Sinha Ray S (2014) Synthesis of nanomaterials by continuous-flow microfluidics: a review. J Nanosci Nanotechnol 14:1338–1363Google Scholar
- 18.Chen-HsunWeng C-C, Huang C-S, Yeh H-Y, Lei G-B (2008) Lee. Synthesis of hexagonal gold nanoparticles using a microfluidic reaction system. J Micromech Microeng 18:1–8Google Scholar
- 22.Liu G, Ma X, Sun X, Jia Y, Wang T (2018) Controllable synthesis of silver nanoparticles using three-phase flow pulsating mixing microfluidic chip. Adv Mater Sci Eng 2018:1–14Google Scholar
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.